#------------------------------------------------------------------------------
#$Date: 2023-12-22 17:07:40 +0200 (Fri, 22 Dec 2023) $
#$Revision: 288505 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/03/31/7033134.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7033134
loop_
_publ_author_name
'Kim, Minsung'
'Kobayashi, Makoto'
'Kato, Hideki'
'Yamane, Hisanori'
'Sato, Yasushi'
'Kakihana, Masato'
_publ_section_title
;
 Crystal structures and luminescence properties of
 Eu²⁺-activated new NaBa0.5Ca0.5PO₄ and
 Na₃Ba₂Ca(PO₄)₃.
;
_journal_issue                   4
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              1900
_journal_page_last               1904
_journal_paper_doi               10.1039/c4dt03024a
_journal_volume                  44
_journal_year                    2015
_chemical_formula_moiety         'Ba2 Ca Na3 O12 P3'
_chemical_formula_structural     'Na2 (Na0.5Ca0.5)2 Ba2 (P O4)3'
_chemical_formula_sum            'Ba2 Ca Na3 O12 P3'
_chemical_formula_weight         668.64
_chemical_name_common
; 
sodium calcium barium phosphate
;
_chemical_name_systematic
; 
Trisodium Monocalcium Dibarium Triphosphorous Dodecaoxygen
;
_space_group_IT_number           159
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      159
_symmetry_space_group_name_Hall  'P 3 -2c'
_symmetry_space_group_name_H-M   'P 3 1 c'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   5.4515(2)
_cell_length_b                   5.4515(2)
_cell_length_c                   23.1283(8)
_cell_measurement_reflns_used    3902
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.45
_cell_measurement_theta_min      3.525
_cell_volume                     595.26(4)
_computing_cell_refinement       'RAPID-AUTO (Rigaku/MSC, 2005)'
_computing_data_collection       'RAPID-AUTO (Rigaku/MSC, 2005)'
_computing_data_reduction        'RAPID-AUTO (Rigaku/MSC, 2005)'
_computing_molecular_graphics    'VESTA (Momma & Izumi, 2008)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SIR2004 (Burla et al., 2005)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 10.0
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Rigaku RAXIS-RAPID II'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71075
_diffrn_reflns_av_R_equivalents  0.0303
_diffrn_reflns_av_sigmaI/netI    0.0215
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       30
_diffrn_reflns_limit_l_min       -30
_diffrn_reflns_number            5929
_diffrn_reflns_theta_full        27.45
_diffrn_reflns_theta_max         27.45
_diffrn_reflns_theta_min         3.52
_exptl_absorpt_coefficient_mu    7.579
_exptl_absorpt_correction_T_max  0.796507
_exptl_absorpt_correction_T_min  0.582105
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details
;
(NUMABS; Higashi, 1999)
;
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    3.730
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       platelet
_exptl_crystal_F_000             612
_exptl_crystal_size_max          0.106
_exptl_crystal_size_mid          0.101
_exptl_crystal_size_min          0.037
_refine_diff_density_max         1.172
_refine_diff_density_min         -0.858
_refine_diff_density_rms         0.166
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.43(18)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.204
_refine_ls_matrix_type           full
_refine_ls_number_parameters     49
_refine_ls_number_reflns         924
_refine_ls_number_restraints     2
_refine_ls_restrained_S_all      1.203
_refine_ls_R_factor_all          0.0388
_refine_ls_R_factor_gt           0.0286
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0254P)²+4.0376P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0659
_refine_ls_wR_factor_ref         0.0744
_reflns_number_gt                756
_reflns_number_total             924
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c4dt03024a2.cif
_cod_data_source_block           Na3CaBa2P3O12
_cod_depositor_comments
;Adding full bibliography for 7033134--7033135.cif.

The following automatic conversions were performed:

data name '_iucr_refine_instruction_details' was replaced with
'_iucr_refine_instructions_details' as specified in the replacement
file 'data/replacement-values/replacement_tags.lst'.

Automatic conversion script
Id: cif_correct_tags 9268 2022-04-12 08:56:07Z antanas 
;
_cod_database_code               7033134
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'y, x, z+1/2'
'-x+y, -x, z'
'-x, -x+y, z+1/2'
'x-y, -y, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Na1 Na 0.3333 0.6667 0.1222(6) 0.012(2) Uani 0.50 3 d SP
Na12 Na 0.3333 0.6667 0.0882(7) 0.012(2) Uani 0.50 3 d SP
Na2 Na 0.3333 0.6667 0.4042(4) 0.0195(10) Uani 0.50 3 d SP
Ca2 Ca 0.3333 0.6667 0.4042(4) 0.0195(10) Uani 0.50 3 d SP
Na3 Na 0.3333 0.6667 0.7102(3) 0.029(3) Uani 1 3 d S
Na4 Na 0.0000 0.0000 0.1591(7) 0.0104(5) Uani 0.50 3 d SP
Ca4 Ca 0.0000 0.0000 0.1591(7) 0.0104(5) Uani 0.50 3 d SP
Ba1 Ba 0.0000 0.0000 -0.00003(4) 0.0222(6) Uani 1 3 d S
Ba2 Ba 0.0000 0.0000 0.31793(2) 0.0200(5) Uani 1 3 d S
P1 P 0.3333 0.6667 0.2441(4) 0.0208(15) Uani 1 3 d S
P2 P 0.3333 0.6667 0.5719(4) 0.0105(12) Uani 1 3 d S
P3 P 0.3333 0.6667 0.88873(19) 0.0158(9) Uani 1 3 d S
O1 O 0.370(2) 0.110(2) 0.0968(4) 0.018(2) Uiso 1 1 d .
O2 O 0.255(3) 0.377(3) 0.2227(5) 0.037(3) Uiso 1 1 d .
O3 O 0.3629(11) 0.1412(15) 0.4088(6) 0.0225(14) Uiso 1 1 d .
O4 O 0.3333 0.6667 0.3096(9) 0.055(3) Uani 1 3 d S
O5 O 0.3333 0.6667 0.5060(10) 0.055(3) Uani 1 3 d S
O6 O 0.3333 0.6667 0.8218(6) 0.020(2) Uani 1 3 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
-0.20 -0.22 23.07 0.0152
-0.47 0.92 -22.80 0.0137
0.20 0.22 -23.07 0.0152
1.88 -5.36 -1.18 0.0446
-3.62 -1.70 -1.75 0.0378
-5.35 3.56 -0.55 0.0241
-1.83 5.35 1.20 0.0287
1.63 3.67 1.76 0.0418
5.43 -2.50 0.94 0.0445
4.62 -4.81 -0.10 0.0353
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Na12 Na1 O1 75.8(4) . 2
Na12 Na1 O1 75.8(4) . 1_565
O1 Na1 O1 114.2(3) 2 1_565
Na12 Na1 O1 75.8(4) . 4_665
O1 Na1 O1 114.2(3) 2 4_665
O1 Na1 O1 114.2(3) 1_565 4_665
Na12 Na1 O2 148.6(3) . 4_565
O1 Na1 O2 92.5(4) 2 4_565
O1 Na1 O2 83.1(3) 1_565 4_565
O1 Na1 O2 134.8(6) 4_665 4_565
Na12 Na1 O2 148.6(3) . 2_665
O1 Na1 O2 134.8(6) 2 2_665
O1 Na1 O2 92.5(4) 1_565 2_665
O1 Na1 O2 83.1(3) 4_665 2_665
O2 Na1 O2 53.6(5) 4_565 2_665
Na12 Na1 O2 148.6(3) . .
O1 Na1 O2 83.1(3) 2 .
O1 Na1 O2 134.8(6) 1_565 .
O1 Na1 O2 92.5(4) 4_665 .
O2 Na1 O2 53.6(5) 4_565 .
O2 Na1 O2 53.6(5) 2_665 .
Na12 Na1 P1 180.000(2) . .
O1 Na1 P1 104.2(4) 2 .
O1 Na1 P1 104.2(4) 1_565 .
O1 Na1 P1 104.2(4) 4_665 .
O2 Na1 P1 31.4(3) 4_565 .
O2 Na1 P1 31.4(3) 2_665 .
O2 Na1 P1 31.4(3) . .
Na12 Na1 Ca4 105.2(3) . 1_565
O1 Na1 Ca4 89.6(3) 2 1_565
O1 Na1 Ca4 44.9(3) 1_565 1_565
O1 Na1 Ca4 155.2(3) 4_665 1_565
O2 Na1 Ca4 44.9(4) 4_565 1_565
O2 Na1 Ca4 84.7(4) 2_665 1_565
O2 Na1 Ca4 97.6(5) . 1_565
P1 Na1 Ca4 74.8(3) . 1_565
Na12 Na1 Na4 105.2(3) . 1_565
O1 Na1 Na4 89.6(3) 2 1_565
O1 Na1 Na4 44.9(3) 1_565 1_565
O1 Na1 Na4 155.2(3) 4_665 1_565
O2 Na1 Na4 44.9(4) 4_565 1_565
O2 Na1 Na4 84.7(4) 2_665 1_565
O2 Na1 Na4 97.6(5) . 1_565
P1 Na1 Na4 74.8(3) . 1_565
Ca4 Na1 Na4 0.0(5) 1_565 1_565
Na12 Na1 Na4 105.2(3) . .
O1 Na1 Na4 44.9(3) 2 .
O1 Na1 Na4 155.2(3) 1_565 .
O1 Na1 Na4 89.6(3) 4_665 .
O2 Na1 Na4 84.7(4) 4_565 .
O2 Na1 Na4 97.6(5) 2_665 .
O2 Na1 Na4 44.9(4) . .
P1 Na1 Na4 74.8(3) . .
Ca4 Na1 Na4 113.4(3) 1_565 .
Na4 Na1 Na4 113.4(3) 1_565 .
Na1 Na12 O1 85.1(4) . 1_565
Na1 Na12 O1 85.1(4) . 2
O1 Na12 O1 119.28(12) 1_565 2
Na1 Na12 O1 85.1(4) . 4_665
O1 Na12 O1 119.28(12) 1_565 4_665
O1 Na12 O1 119.28(12) 2 4_665
Na1 Na12 P2 96.8(3) . 3_554
O1 Na12 P2 145.8(3) 1_565 3_554
O1 Na12 P2 94.9(3) 2 3_554
O1 Na12 P2 28.2(3) 4_665 3_554
Na1 Na12 P2 96.8(3) . 3_454
O1 Na12 P2 94.9(3) 1_565 3_454
O1 Na12 P2 28.2(3) 2 3_454
O1 Na12 P2 145.8(3) 4_665 3_454
P2 Na12 P2 118.62(14) 3_554 3_454
Na1 Na12 P2 96.8(3) . 3_564
O1 Na12 P2 28.2(3) 1_565 3_564
O1 Na12 P2 145.8(3) 2 3_564
O1 Na12 P2 94.9(3) 4_665 3_564
P2 Na12 P2 118.62(14) 3_554 3_564
P2 Na12 P2 118.62(14) 3_454 3_564
Na1 Na12 Na4 62.5(4) . .
O1 Na12 Na4 139.2(6) 1_565 .
O1 Na12 Na4 39.7(3) 2 .
O1 Na12 Na4 83.9(3) 4_665 .
P2 Na12 Na4 67.32(11) 3_554 .
P2 Na12 Na4 67.32(11) 3_454 .
P2 Na12 Na4 159.3(7) 3_564 .
Na1 Na12 Ca4 62.5(4) . 1_565
O1 Na12 Ca4 39.7(3) 1_565 1_565
O1 Na12 Ca4 83.9(3) 2 1_565
O1 Na12 Ca4 139.2(6) 4_665 1_565
P2 Na12 Ca4 159.3(7) 3_554 1_565
P2 Na12 Ca4 67.32(11) 3_454 1_565
P2 Na12 Ca4 67.32(11) 3_564 1_565
Na4 Na12 Ca4 100.4(5) . 1_565
Na1 Na12 Na4 62.5(4) . 1_565
O1 Na12 Na4 39.7(3) 1_565 1_565
O1 Na12 Na4 83.9(3) 2 1_565
O1 Na12 Na4 139.2(6) 4_665 1_565
P2 Na12 Na4 159.3(7) 3_554 1_565
P2 Na12 Na4 67.32(11) 3_454 1_565
P2 Na12 Na4 67.32(11) 3_564 1_565
Na4 Na12 Na4 100.4(5) . 1_565
Ca4 Na12 Na4 0.0(5) 1_565 1_565
Na1 Na12 Ca4 62.5(4) . 1_665
O1 Na12 Ca4 83.9(3) 1_565 1_665
O1 Na12 Ca4 139.2(6) 2 1_665
O1 Na12 Ca4 39.7(3) 4_665 1_665
P2 Na12 Ca4 67.32(11) 3_554 1_665
P2 Na12 Ca4 159.3(7) 3_454 1_665
P2 Na12 Ca4 67.32(11) 3_564 1_665
Na4 Na12 Ca4 100.4(5) . 1_665
Ca4 Na12 Ca4 100.4(5) 1_565 1_665
Na4 Na12 Ca4 100.4(5) 1_565 1_665
O4 Na2 O5 180.000(5) . .
O4 Na2 O3 92.4(3) . 1_565
O5 Na2 O3 87.6(3) . 1_565
O4 Na2 O3 92.4(3) . 2
O5 Na2 O3 87.6(3) . 2
O3 Na2 O3 119.82(5) 1_565 2
O4 Na2 O3 92.4(3) . 4_665
O5 Na2 O3 87.6(3) . 4_665
O3 Na2 O3 119.82(5) 1_565 4_665
O3 Na2 O3 119.82(5) 2 4_665
O4 Na2 O3 92.1(3) . 4_565
O5 Na2 O3 87.9(3) . 4_565
O3 Na2 O3 65.9(2) 1_565 4_565
O3 Na2 O3 54.0(2) 2 4_565
O3 Na2 O3 172.6(4) 4_665 4_565
O4 Na2 O3 92.1(3) . 2_665
O5 Na2 O3 87.9(3) . 2_665
O3 Na2 O3 54.0(2) 1_565 2_665
O3 Na2 O3 172.6(4) 2 2_665
O3 Na2 O3 65.9(2) 4_665 2_665
O3 Na2 O3 119.87(4) 4_565 2_665
O4 Na2 O3 92.1(3) . .
O5 Na2 O3 87.9(3) . .
O3 Na2 O3 172.6(4) 1_565 .
O3 Na2 O3 65.9(2) 2 .
O3 Na2 O3 54.0(2) 4_665 .
O3 Na2 O3 119.87(4) 4_565 .
O3 Na2 O3 119.87(4) 2_665 .
O4 Na2 P3 83.52(17) . 3_554
O5 Na2 P3 96.48(17) . 3_554
O3 Na2 P3 146.67(13) 1_565 3_554
O3 Na2 P3 93.44(13) 2 3_554
O3 Na2 P3 28.21(14) 4_665 3_554
O3 Na2 P3 147.09(11) 4_565 3_554
O3 Na2 P3 92.93(11) 2_665 3_554
O3 Na2 P3 28.55(12) . 3_554
O4 Na2 P3 83.52(17) . 3_454
O5 Na2 P3 96.48(17) . 3_454
O3 Na2 P3 93.44(13) 1_565 3_454
O3 Na2 P3 28.21(14) 2 3_454
O3 Na2 P3 146.67(13) 4_665 3_454
O3 Na2 P3 28.55(12) 4_565 3_454
O3 Na2 P3 147.09(11) 2_665 3_454
O3 Na2 P3 92.93(11) . 3_454
P3 Na2 P3 118.74(7) 3_554 3_454
O4 Na2 P3 83.52(17) . 3_564
O5 Na2 P3 96.48(17) . 3_564
O3 Na2 P3 28.21(14) 1_565 3_564
O3 Na2 P3 146.67(13) 2 3_564
O3 Na2 P3 93.45(13) 4_665 3_564
O3 Na2 P3 92.93(11) 4_565 3_564
O3 Na2 P3 28.55(12) 2_665 3_564
O3 Na2 P3 147.09(12) . 3_564
P3 Na2 P3 118.74(7) 3_554 3_564
P3 Na2 P3 118.74(7) 3_454 3_564
O4 Na2 Ba2 57.63(11) . 1_565
O5 Na2 Ba2 122.37(11) . 1_565
O3 Na2 Ba2 46.9(3) 1_565 1_565
O3 Na2 Ba2 88.6(2) 2 1_565
O3 Na2 Ba2 140.9(3) 4_665 1_565
O3 Na2 Ba2 46.3(2) 4_565 1_565
O3 Na2 Ba2 88.82(17) 2_665 1_565
O3 Na2 Ba2 140.3(3) . 1_565
P3 Na2 Ba2 141.2(3) 3_554 1_565
P3 Na2 Ba2 61.31(8) 3_454 1_565
P3 Na2 Ba2 61.31(8) 3_564 1_565
O2 Na3 O2 118.56(15) 3 5_665
O2 Na3 O2 118.56(15) 3 6_565
O2 Na3 O2 118.56(14) 5_665 6_565
O2 Na3 O6 83.1(3) 3 .
O2 Na3 O6 83.1(3) 5_665 .
O2 Na3 O6 83.1(3) 6_565 .
O2 Na3 O1 78.7(3) 3 3
O2 Na3 O1 125.6(5) 5_665 3
O2 Na3 O1 86.1(4) 6_565 3
O6 Na3 O1 151.0(2) . 3
O2 Na3 O1 125.6(5) 3 6_565
O2 Na3 O1 86.1(4) 5_665 6_565
O2 Na3 O1 78.7(3) 6_565 6_565
O6 Na3 O1 151.0(2) . 6_565
O1 Na3 O1 49.7(4) 3 6_565
O2 Na3 O1 86.1(4) 3 5_665
O2 Na3 O1 78.7(3) 5_665 5_665
O2 Na3 O1 125.6(5) 6_565 5_665
O6 Na3 O1 151.0(2) . 5_665
O1 Na3 O1 49.7(4) 3 5_665
O1 Na3 O1 49.7(4) 6_565 5_665
O2 Na3 P2 96.9(3) 3 .
O2 Na3 P2 96.9(3) 5_665 .
O2 Na3 P2 96.9(3) 6_565 .
O6 Na3 P2 180.000(3) . .
O1 Na3 P2 29.0(2) 3 .
O1 Na3 P2 29.0(2) 6_565 .
O1 Na3 P2 29.0(2) 5_665 .
O2 Na3 P1 25.6(3) 3 3
O2 Na3 P1 93.1(3) 5_665 3
O2 Na3 P1 139.5(3) 6_565 3
O6 Na3 P1 76.02(17) . 3
O1 Na3 P1 95.7(2) 3 3
O1 Na3 P1 131.6(3) 6_565 3
O1 Na3 P1 82.6(2) 5_665 3
P2 Na3 P1 103.98(17) . 3
O2 Na3 P1 139.5(4) 3 3_565
O2 Na3 P1 25.6(3) 5_665 3_565
O2 Na3 P1 93.1(3) 6_565 3_565
O6 Na3 P1 76.02(18) . 3_565
O1 Na3 P1 131.6(3) 3 3_565
O1 Na3 P1 82.6(2) 6_565 3_565
O1 Na3 P1 95.7(2) 5_665 3_565
P2 Na3 P1 103.98(17) . 3_565
P1 Na3 P1 114.36(14) 3 3_565
O2 Na3 P1 93.1(3) 3 3_455
O2 Na3 P1 139.5(3) 5_665 3_455
O2 Na3 P1 25.6(3) 6_565 3_455
O6 Na3 P1 76.02(17) . 3_455
O1 Na3 P1 82.6(2) 3 3_455
O1 Na3 P1 95.7(2) 6_565 3_455
O1 Na3 P1 131.6(3) 5_665 3_455
P2 Na3 P1 103.98(18) . 3_455
P1 Na3 P1 114.36(14) 3 3_455
P1 Na3 P1 114.36(13) 3_565 3_455
O2 Na3 Na4 152.2(4) 3 3_565
O2 Na3 Na4 87.8(3) 5_665 3_565
O2 Na3 Na4 44.0(3) 6_565 3_565
O6 Na3 Na4 110.6(3) . 3_565
O1 Na3 Na4 78.5(3) 3 3_565
O1 Na3 Na4 41.9(3) 6_565 3_565
O1 Na3 Na4 91.2(3) 5_665 3_565
P2 Na3 Na4 69.4(3) . 3_565
P1 Na3 Na4 173.4(4) 3 3_565
P1 Na3 Na4 68.33(10) 3_565 3_565
P1 Na3 Na4 68.33(10) 3_455 3_565
O1 Na4 O1 85.0(6) . 4
O1 Na4 O1 85.0(6) . 2
O1 Na4 O1 85.0(6) 4 2
O1 Na4 O2 178.8(6) . 2
O1 Na4 O2 94.4(4) 4 2
O1 Na4 O2 96.0(4) 2 2
O1 Na4 O2 94.4(4) . 4
O1 Na4 O2 96.0(4) 4 4
O1 Na4 O2 178.8(6) 2 4
O2 Na4 O2 84.6(6) 2 4
O1 Na4 O2 96.0(4) . .
O1 Na4 O2 178.8(6) 4 .
O1 Na4 O2 94.4(4) 2 .
O2 Na4 O2 84.6(6) 2 .
O2 Na4 O2 84.6(6) 4 .
O1 Na4 Na1 124.7(7) . 1_445
O1 Na4 Na1 47.3(3) 4 1_445
O1 Na4 Na1 67.5(3) 2 1_445
O2 Na4 Na1 55.3(4) 2 1_445
O2 Na4 Na1 113.7(4) 4 1_445
O2 Na4 Na1 131.5(5) . 1_445
O1 Na4 Na1 67.5(3) . .
O1 Na4 Na1 124.7(7) 4 .
O1 Na4 Na1 47.3(3) 2 .
O2 Na4 Na1 113.7(4) 2 .
O2 Na4 Na1 131.5(5) 4 .
O2 Na4 Na1 55.3(4) . .
Na1 Na4 Na1 113.4(3) 1_445 .
O1 Na4 Na1 47.3(3) . 1_545
O1 Na4 Na1 67.5(3) 4 1_545
O1 Na4 Na1 124.7(7) 2 1_545
O2 Na4 Na1 131.5(5) 2 1_545
O2 Na4 Na1 55.3(4) 4 1_545
O2 Na4 Na1 113.7(4) . 1_545
Na1 Na4 Na1 113.4(3) 1_445 1_545
Na1 Na4 Na1 113.4(3) . 1_545
O1 Na4 Na3 60.6(3) . 3_554
O1 Na4 Na3 136.0(3) 4 3_554
O1 Na4 Na3 115.6(3) 2 3_554
O2 Na4 Na3 119.4(6) 2 3_554
O2 Na4 Na3 63.2(4) 4 3_554
O2 Na4 Na3 45.2(3) . 3_554
Na1 Na4 Na3 174.6(6) 1_445 3_554
Na1 Na4 Na3 68.92(11) . 3_554
Na1 Na4 Na3 68.92(11) 1_545 3_554
O1 Na4 Na3 115.6(3) . 3_444
O1 Na4 Na3 60.6(3) 4 3_444
O1 Na4 Na3 136.0(3) 2 3_444
O2 Na4 Na3 63.2(4) 2 3_444
O2 Na4 Na3 45.2(3) 4 3_444
O2 Na4 Na3 119.4(6) . 3_444
Na1 Na4 Na3 68.92(11) 1_445 3_444
Na1 Na4 Na3 174.6(6) . 3_444
Na1 Na4 Na3 68.92(11) 1_545 3_444
Na3 Na4 Na3 108.3(3) 3_554 3_444
O1 Na4 Na3 136.0(3) . 3_454
O1 Na4 Na3 115.6(3) 4 3_454
O1 Na4 Na3 60.6(3) 2 3_454
O2 Na4 Na3 45.2(3) 2 3_454
O2 Na4 Na3 119.4(6) 4 3_454
O2 Na4 Na3 63.2(4) . 3_454
Na1 Na4 Na3 68.92(11) 1_445 3_454
Na1 Na4 Na3 68.92(11) . 3_454
Na1 Na4 Na3 174.6(6) 1_545 3_454
Na3 Na4 Na3 108.3(3) 3_554 3_454
Na3 Na4 Na3 108.3(3) 3_444 3_454
O3 Ba1 O3 66.6(3) 6_554 5_554
O3 Ba1 O3 66.6(3) 6_554 3_554
O3 Ba1 O3 66.6(3) 5_554 3_554
O3 Ba1 O1 167.2(3) 6_554 2
O3 Ba1 O1 122.5(3) 5_554 2
O3 Ba1 O1 107.3(3) 3_554 2
O3 Ba1 O1 122.5(3) 6_554 4
O3 Ba1 O1 107.3(3) 5_554 4
O3 Ba1 O1 167.2(3) 3_554 4
O1 Ba1 O1 65.6(3) 2 4
O3 Ba1 O1 107.3(3) 6_554 .
O3 Ba1 O1 167.2(3) 5_554 .
O3 Ba1 O1 122.5(3) 3_554 .
O1 Ba1 O1 65.6(3) 2 .
O1 Ba1 O1 65.6(3) 4 .
O3 Ba1 O5 69.6(4) 6_554 3_554
O3 Ba1 O5 131.5(5) 5_554 3_554
O3 Ba1 O5 77.9(4) 3_554 3_554
O1 Ba1 O5 98.4(4) 2 3_554
O1 Ba1 O5 113.1(5) 4 3_554
O1 Ba1 O5 49.9(4) . 3_554
O3 Ba1 O5 77.9(4) 6_554 3_444
O3 Ba1 O5 69.6(4) 5_554 3_444
O3 Ba1 O5 131.5(5) 3_554 3_444
O1 Ba1 O5 113.1(5) 2 3_444
O1 Ba1 O5 49.9(4) 4 3_444
O1 Ba1 O5 98.4(4) . 3_444
O5 Ba1 O5 119.81(7) 3_554 3_444
O3 Ba1 O5 131.5(5) 6_554 3_454
O3 Ba1 O5 77.9(4) 5_554 3_454
O3 Ba1 O5 69.6(4) 3_554 3_454
O1 Ba1 O5 49.9(4) 2 3_454
O1 Ba1 O5 98.4(4) 4 3_454
O1 Ba1 O5 113.1(5) . 3_454
O5 Ba1 O5 119.80(7) 3_554 3_454
O5 Ba1 O5 119.80(7) 3_444 3_454
O3 Ba1 P2 91.3(2) 6_554 3_554
O3 Ba1 P2 156.5(3) 5_554 3_554
O3 Ba1 P2 98.36(19) 3_554 3_554
O1 Ba1 P2 78.2(2) 2 3_554
O1 Ba1 P2 90.8(2) 4 3_554
O1 Ba1 P2 25.4(2) . 3_554
O5 Ba1 P2 25.3(4) 3_554 3_554
O5 Ba1 P2 114.9(3) 3_444 3_554
O5 Ba1 P2 114.9(3) 3_454 3_554
O3 Ba1 P2 98.37(19) 6_554 3_444
O3 Ba1 P2 91.3(2) 5_554 3_444
O3 Ba1 P2 156.5(3) 3_554 3_444
O1 Ba1 P2 90.8(2) 2 3_444
O1 Ba1 P2 25.4(2) 4 3_444
O1 Ba1 P2 78.2(2) . 3_444
O5 Ba1 P2 114.9(3) 3_554 3_444
O5 Ba1 P2 25.3(4) 3_444 3_444
O5 Ba1 P2 114.9(3) 3_454 3_444
P2 Ba1 P2 99.92(17) 3_554 3_444
O3 Ba1 P2 156.5(3) 6_554 3_454
O3 Ba1 P2 98.36(19) 5_554 3_454
O3 Ba1 P2 91.3(2) 3_554 3_454
O1 Ba1 P2 25.4(2) 2 3_454
O1 Ba1 P2 78.2(2) 4 3_454
O1 Ba1 P2 90.8(2) . 3_454
O5 Ba1 P2 114.9(3) 3_554 3_454
O5 Ba1 P2 114.9(3) 3_444 3_454
O5 Ba1 P2 25.3(4) 3_454 3_454
P2 Ba1 P2 99.92(17) 3_554 3_454
P2 Ba1 P2 99.92(17) 3_444 3_454
O3 Ba2 O3 66.7(3) 2 4
O3 Ba2 O3 66.7(3) 2 .
O3 Ba2 O3 66.7(3) 4 .
O3 Ba2 O2 114.9(3) 2 .
O3 Ba2 O2 177.3(4) 4 .
O3 Ba2 O2 111.6(3) . .
O3 Ba2 O2 111.6(3) 2 2
O3 Ba2 O2 114.9(3) 4 2
O3 Ba2 O2 177.3(4) . 2
O2 Ba2 O2 66.9(4) . 2
O3 Ba2 O2 177.3(4) 2 4
O3 Ba2 O2 111.6(3) 4 4
O3 Ba2 O2 114.9(3) . 4
O2 Ba2 O2 66.9(4) . 4
O2 Ba2 O2 66.9(4) 2 4
O3 Ba2 O6 102.9(3) 2 3_554
O3 Ba2 O6 111.3(3) 4 3_554
O3 Ba2 O6 49.3(3) . 3_554
O2 Ba2 O6 66.4(3) . 3_554
O2 Ba2 O6 130.2(3) 2 3_554
O2 Ba2 O6 79.7(3) 4 3_554
O3 Ba2 O6 111.3(3) 2 3_444
O3 Ba2 O6 49.3(3) 4 3_444
O3 Ba2 O6 102.9(3) . 3_444
O2 Ba2 O6 130.2(3) . 3_444
O2 Ba2 O6 79.7(3) 2 3_444
O2 Ba2 O6 66.4(3) 4 3_444
O6 Ba2 O6 119.92(2) 3_554 3_444
O3 Ba2 O6 49.3(3) 2 3_454
O3 Ba2 O6 102.9(3) 4 3_454
O3 Ba2 O6 111.3(3) . 3_454
O2 Ba2 O6 79.7(3) . 3_454
O2 Ba2 O6 66.4(3) 2 3_454
O2 Ba2 O6 130.2(3) 4 3_454
O6 Ba2 O6 119.92(2) 3_554 3_454
O6 Ba2 O6 119.92(2) 3_444 3_454
O3 Ba2 O4 78.6(3) 2 1_445
O3 Ba2 O4 70.3(3) 4 1_445
O3 Ba2 O4 132.5(5) . 1_445
O2 Ba2 O4 112.0(4) . 1_445
O2 Ba2 O4 48.0(4) 2 1_445
O2 Ba2 O4 98.8(4) 4 1_445
O6 Ba2 O4 178.1(6) 3_554 1_445
O6 Ba2 O4 60.19(2) 3_444 1_445
O6 Ba2 O4 60.19(2) 3_454 1_445
O3 Ba2 O4 70.3(3) 2 .
O3 Ba2 O4 132.5(5) 4 .
O3 Ba2 O4 78.6(3) . .
O2 Ba2 O4 48.0(4) . .
O2 Ba2 O4 98.8(4) 2 .
O2 Ba2 O4 112.0(4) 4 .
O6 Ba2 O4 60.19(2) 3_554 .
O6 Ba2 O4 178.1(6) 3_444 .
O6 Ba2 O4 60.19(2) 3_454 .
O4 Ba2 O4 119.63(8) 1_445 .
O3 Ba2 O4 132.5(5) 2 1_545
O3 Ba2 O4 78.6(3) 4 1_545
O3 Ba2 O4 70.3(3) . 1_545
O2 Ba2 O4 98.8(4) . 1_545
O2 Ba2 O4 112.0(4) 2 1_545
O2 Ba2 O4 48.0(4) 4 1_545
O6 Ba2 O4 60.19(2) 3_554 1_545
O6 Ba2 O4 60.19(2) 3_444 1_545
O6 Ba2 O4 178.1(6) 3_454 1_545
O4 Ba2 O4 119.63(8) 1_445 1_545
O4 Ba2 O4 119.63(8) . 1_545
O2 P1 O2 109.7(5) . 4_565
O2 P1 O2 109.7(5) . 2_665
O2 P1 O2 109.7(5) 4_565 2_665
O2 P1 O4 109.3(5) . .
O2 P1 O4 109.3(5) 4_565 .
O2 P1 O4 109.3(5) 2_665 .
O2 P1 Na1 70.7(5) . .
O2 P1 Na1 70.7(5) 4_565 .
O2 P1 Na1 70.7(5) 2_665 .
O4 P1 Na1 180.000(2) . .
O2 P1 Na3 43.4(5) . 3_554
O2 P1 Na3 143.7(6) 4_565 3_554
O2 P1 Na3 71.5(5) 2_665 3_554
O4 P1 Na3 103.98(17) . 3_554
Na1 P1 Na3 76.02(17) . 3_554
O2 P1 Na3 71.5(5) . 3_454
O2 P1 Na3 43.4(5) 4_565 3_454
O2 P1 Na3 143.7(6) 2_665 3_454
O4 P1 Na3 103.98(17) . 3_454
Na1 P1 Na3 76.02(17) . 3_454
Na3 P1 Na3 114.36(13) 3_554 3_454
O2 P1 Na3 143.7(6) . 3_564
O2 P1 Na3 71.5(5) 4_565 3_564
O2 P1 Na3 43.4(5) 2_665 3_564
O4 P1 Na3 103.98(17) . 3_564
Na1 P1 Na3 76.02(17) . 3_564
Na3 P1 Na3 114.36(13) 3_554 3_564
Na3 P1 Na3 114.36(13) 3_454 3_564
O2 P1 Ba2 49.9(5) . .
O2 P1 Ba2 111.9(5) 4_565 .
O2 P1 Ba2 138.0(5) 2_665 .
O4 P1 Ba2 61.51(13) . .
Na1 P1 Ba2 118.49(13) . .
Na3 P1 Ba2 71.87(8) 3_554 .
Na3 P1 Ba2 71.87(8) 3_454 .
Na3 P1 Ba2 165.5(3) 3_564 .
O2 P1 Ba2 138.0(5) . 1_565
O2 P1 Ba2 49.9(5) 4_565 1_565
O2 P1 Ba2 111.9(5) 2_665 1_565
O4 P1 Ba2 61.51(13) . 1_565
Na1 P1 Ba2 118.49(13) . 1_565
Na3 P1 Ba2 165.5(3) 3_554 1_565
Na3 P1 Ba2 71.87(8) 3_454 1_565
Na3 P1 Ba2 71.87(8) 3_564 1_565
Ba2 P1 Ba2 99.13(16) . 1_565
O2 P1 Ba2 111.9(5) . 1_665
O2 P1 Ba2 138.0(5) 4_565 1_665
O2 P1 Ba2 49.9(5) 2_665 1_665
O4 P1 Ba2 61.51(13) . 1_665
Na1 P1 Ba2 118.49(13) . 1_665
Na3 P1 Ba2 71.87(8) 3_554 1_665
Na3 P1 Ba2 165.5(3) 3_454 1_665
Na3 P1 Ba2 71.87(8) 3_564 1_665
Ba2 P1 Ba2 99.13(16) . 1_665
Ba2 P1 Ba2 99.13(16) 1_565 1_665
O5 P2 O1 111.5(5) . 6_565
O5 P2 O1 111.5(5) . 3
O1 P2 O1 107.4(5) 6_565 3
O5 P2 O1 111.5(5) . 5_665
O1 P2 O1 107.4(5) 6_565 5_665
O1 P2 O1 107.4(5) 3 5_665
O5 P2 Na12 96.8(3) . 3
O1 P2 Na12 147.5(6) 6_565 3
O1 P2 Na12 74.8(4) 3 3
O1 P2 Na12 44.7(4) 5_665 3
O5 P2 Na12 96.8(3) . 3_565
O1 P2 Na12 44.7(4) 6_565 3_565
O1 P2 Na12 147.5(6) 3 3_565
O1 P2 Na12 74.8(4) 5_665 3_565
Na12 P2 Na12 118.62(14) 3 3_565
O5 P2 Na12 96.8(3) . 3_455
O1 P2 Na12 74.8(4) 6_565 3_455
O1 P2 Na12 44.7(4) 3 3_455
O1 P2 Na12 147.5(6) 5_665 3_455
Na12 P2 Na12 118.62(14) 3 3_455
Na12 P2 Na12 118.62(14) 3_565 3_455
O5 P2 Na3 180.000(4) . .
O1 P2 Na3 68.5(5) 6_565 .
O1 P2 Na3 68.5(5) 3 .
O1 P2 Na3 68.5(5) 5_665 .
Na12 P2 Na3 83.2(3) 3 .
Na12 P2 Na3 83.2(3) 3_565 .
Na12 P2 Na3 83.2(3) 3_455 .
O5 P2 Na1 110.3(2) . 3
O1 P2 Na1 135.3(5) 6_565 3
O1 P2 Na1 70.5(4) 3 3
O1 P2 Na1 40.7(4) 5_665 3
Na12 P2 Na1 13.5(4) 3 3
Na12 P2 Na1 115.13(18) 3_565 3
Na12 P2 Na1 115.13(18) 3_455 3
Na3 P2 Na1 69.7(2) . 3
O5 P2 Na1 110.3(2) . 3_565
O1 P2 Na1 40.7(4) 6_565 3_565
O1 P2 Na1 135.3(5) 3 3_565
O1 P2 Na1 70.5(4) 5_665 3_565
Na12 P2 Na1 115.13(18) 3 3_565
Na12 P2 Na1 13.5(4) 3_565 3_565
Na12 P2 Na1 115.13(18) 3_455 3_565
Na3 P2 Na1 69.7(2) . 3_565
Na1 P2 Na1 108.7(2) 3 3_565
O5 P2 Na1 110.3(2) . 3_455
O1 P2 Na1 70.5(4) 6_565 3_455
O1 P2 Na1 40.7(4) 3 3_455
O1 P2 Na1 135.3(5) 5_665 3_455
Na12 P2 Na1 115.13(18) 3 3_455
Na12 P2 Na1 115.13(18) 3_565 3_455
Na12 P2 Na1 13.5(4) 3_455 3_455
Na3 P2 Na1 69.7(2) . 3_455
Na1 P2 Na1 108.7(2) 3 3_455
Na1 P2 Na1 108.7(2) 3_565 3_455
O5 P2 Ba1 62.13(13) . 3_565
O1 P2 Ba1 51.8(4) 6_565 3_565
O1 P2 Ba1 111.5(4) 3 3_565
O1 P2 Ba1 140.0(4) 5_665 3_565
Na12 P2 Ba1 158.9(4) 3 3_565
Na12 P2 Ba1 67.45(17) 3_565 3_565
Na12 P2 Ba1 67.45(17) 3_455 3_565
Na3 P2 Ba1 117.87(13) . 3_565
Na1 P2 Ba1 172.4(3) 3 3_565
Na1 P2 Ba1 75.36(12) 3_565 3_565
Na1 P2 Ba1 75.36(12) 3_455 3_565
O3 P3 O3 111.1(5) 5_665 3
O3 P3 O3 111.1(5) 5_665 6_565
O3 P3 O3 111.1(5) 3 6_565
O3 P3 O6 107.7(5) 5_665 .
O3 P3 O6 107.7(5) 3 .
O3 P3 O6 107.7(5) 6_565 .
O3 P3 Na2 51.2(3) 5_665 3
O3 P3 Na2 67.8(3) 3 3
O3 P3 Na2 154.3(6) 6_565 3
O6 P3 Na2 96.48(17) . 3
O3 P3 Ca2 51.2(3) 5_665 3
O3 P3 Ca2 67.8(3) 3 3
O3 P3 Ca2 154.3(6) 6_565 3
O6 P3 Ca2 96.48(17) . 3
Na2 P3 Ca2 0.0(3) 3 3
O3 P3 Na2 67.8(3) 5_665 3_565
O3 P3 Na2 154.3(6) 3 3_565
O3 P3 Na2 51.2(3) 6_565 3_565
O6 P3 Na2 96.48(17) . 3_565
Na2 P3 Na2 118.75(7) 3 3_565
Ca2 P3 Na2 118.75(7) 3 3_565
O3 P3 Ca2 67.8(3) 5_665 3_565
O3 P3 Ca2 154.3(6) 3 3_565
O3 P3 Ca2 51.2(3) 6_565 3_565
O6 P3 Ca2 96.48(17) . 3_565
Na2 P3 Ca2 118.75(7) 3 3_565
Ca2 P3 Ca2 118.75(7) 3 3_565
Na2 P3 Ca2 0.0(3) 3_565 3_565
O3 P3 Ca2 154.3(6) 5_665 3_455
O3 P3 Ca2 51.2(3) 3 3_455
O3 P3 Ca2 67.8(3) 6_565 3_455
O6 P3 Ca2 96.48(17) . 3_455
Na2 P3 Ca2 118.75(7) 3 3_455
Ca2 P3 Ca2 118.75(7) 3 3_455
Na2 P3 Ca2 118.74(7) 3_565 3_455
Ca2 P3 Ca2 118.74(7) 3_565 3_455
O3 P3 Na2 154.3(6) 5_665 3_455
O3 P3 Na2 51.2(3) 3 3_455
O3 P3 Na2 67.8(3) 6_565 3_455
O6 P3 Na2 96.48(17) . 3_455
Na2 P3 Na2 118.75(7) 3 3_455
Ca2 P3 Na2 118.75(7) 3 3_455
Na2 P3 Na2 118.74(7) 3_565 3_455
Ca2 P3 Na2 118.74(7) 3_565 3_455
Ca2 P3 Na2 0.0 3_455 3_455
O3 P3 Ba2 132.0(3) 5_665 3_565
O3 P3 Ba2 116.6(3) 3 3_565
O3 P3 Ba2 46.0(5) 6_565 3_565
O6 P3 Ba2 62.52(7) . 3_565
Na2 P3 Ba2 159.0(2) 3 3_565
Ca2 P3 Ba2 159.0(2) 3 3_565
Na2 P3 Ba2 67.13(9) 3_565 3_565
Ca2 P3 Ba2 67.13(9) 3_565 3_565
Ca2 P3 Ba2 67.13(9) 3_455 3_565
Na2 P3 Ba2 67.13(9) 3_455 3_565
O3 P3 Ba2 116.6(3) 5_665 3
O3 P3 Ba2 46.0(5) 3 3
O3 P3 Ba2 132.0(3) 6_565 3
O6 P3 Ba2 62.52(7) . 3
Na2 P3 Ba2 67.13(9) 3 3
Ca2 P3 Ba2 67.13(9) 3 3
Na2 P3 Ba2 159.0(2) 3_565 3
Ca2 P3 Ba2 159.0(2) 3_565 3
Ca2 P3 Ba2 67.13(9) 3_455 3
Na2 P3 Ba2 67.13(9) 3_455 3
Ba2 P3 Ba2 100.40(8) 3_565 3
P2 O1 Na4 149.5(6) 3_554 .
P2 O1 Na12 107.1(5) 3_554 1_545
Na4 O1 Na12 99.9(4) . 1_545
P2 O1 Na1 114.0(5) 3_554 1_545
Na4 O1 Na1 87.8(4) . 1_545
Na12 O1 Na1 19.1(5) 1_545 1_545
P2 O1 Ba1 102.8(5) 3_554 .
Na4 O1 Ba1 90.0(5) . .
Na12 O1 Ba1 91.7(4) 1_545 .
Na1 O1 Ba1 106.5(4) 1_545 .
P2 O1 Na3 82.5(5) 3_554 3_554
Na4 O1 Na3 77.5(4) . 3_554
Na12 O1 Na3 104.2(4) 1_545 3_554
Na1 O1 Na3 87.2(4) 1_545 3_554
Ba1 O1 Na3 161.2(4) . 3_554
P1 O2 Na4 149.7(8) . .
P1 O2 Na3 111.1(6) . 3_554
Na4 O2 Na3 90.8(5) . 3_554
P1 O2 Na1 77.9(6) . .
Na4 O2 Na1 79.9(4) . .
Na3 O2 Na1 94.2(4) 3_554 .
P1 O2 Ba2 106.4(6) . .
Na4 O2 Ba2 89.5(5) . .
Na3 O2 Ba2 99.6(5) 3_554 .
Na1 O2 Ba2 162.7(5) . .
P3 O3 Ca2 100.6(3) 3_554 1_545
P3 O3 Na2 100.6(3) 3_554 1_545
Ca2 O3 Na2 0.0(4) 1_545 1_545
P3 O3 Ba2 110.2(7) 3_554 .
Ca2 O3 Ba2 90.7(3) 1_545 .
Na2 O3 Ba2 90.7(3) 1_545 .
P3 O3 Ba1 144.7(7) 3_554 3
Ca2 O3 Ba1 94.5(3) 1_545 3
Na2 O3 Ba1 94.5(3) 1_545 3
Ba2 O3 Ba1 101.26(17) . 3
P3 O3 Na2 83.7(3) 3_554 .
Ca2 O3 Na2 172.6(4) 1_545 .
Na2 O3 Na2 172.6(4) 1_545 .
Ba2 O3 Na2 82.0(3) . .
Ba1 O3 Na2 85.3(2) 3 .
P1 O4 Na2 180.000(2) . .
P1 O4 Ba2 93.5(4) . 1_565
Na2 O4 Ba2 86.5(4) . 1_565
P1 O4 Ba2 93.5(4) . .
Na2 O4 Ba2 86.5(4) . .
Ba2 O4 Ba2 119.63(8) 1_565 .
P1 O4 Ba2 93.5(4) . 1_665
Na2 O4 Ba2 86.5(4) . 1_665
Ba2 O4 Ba2 119.63(8) 1_565 1_665
Ba2 O4 Ba2 119.63(8) . 1_665
P2 O5 Na2 180.000(2) . .
P2 O5 Ba1 92.5(4) . 3_565
Na2 O5 Ba1 87.5(4) . 3_565
P2 O5 Ba1 92.5(4) . 3
Na2 O5 Ba1 87.5(4) . 3
Ba1 O5 Ba1 119.80(7) 3_565 3
P2 O5 Ba1 92.5(4) . 3_665
Na2 O5 Ba1 87.5(4) . 3_665
Ba1 O5 Ba1 119.80(7) 3_565 3_665
Ba1 O5 Ba1 119.80(7) 3 3_665
P3 O6 Na3 180.000(3) . .
P3 O6 Ba2 91.6(2) . 3_565
Na3 O6 Ba2 88.4(2) . 3_565
P3 O6 Ba2 91.6(2) . 3_665
Na3 O6 Ba2 88.4(2) . 3_665
Ba2 O6 Ba2 119.92(2) 3_565 3_665
P3 O6 Ba2 91.6(2) . 3
Na3 O6 Ba2 88.4(2) . 3
Ba2 O6 Ba2 119.92(2) 3_565 3
Ba2 O6 Ba2 119.92(2) 3_665 3
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Na1 Na12 0.79(2) .
Na1 O1 2.398(10) 2
Na1 O1 2.398(10) 1_565
Na1 O1 2.398(10) 4_665
Na1 O2 2.722(16) 4_565
Na1 O2 2.722(16) 2_665
Na1 O2 2.722(16) .
Na1 P1 2.819(14) .
Na1 Ca4 3.261(5) 1_565
Na1 Na4 3.261(5) 1_565
Na1 Na4 3.261(5) .
Na12 O1 2.333(10) 1_565
Na12 O1 2.333(10) 2
Na12 O1 2.333(10) 4_665
Na12 P2 3.170(2) 3_554
Na12 P2 3.170(2) 3_454
Na12 P2 3.170(2) 3_564
Na12 Na4 3.549(12) .
Na12 Ca4 3.549(12) 1_565
Na12 Na4 3.549(12) 1_565
Na12 Ca4 3.549(12) 1_665
Na2 O4 2.19(2) .
Na2 O5 2.36(2) .
Na2 O3 2.512(7) 1_565
Na2 O3 2.512(8) 2
Na2 O3 2.512(7) 4_665
Na2 O3 2.951(8) 4_565
Na2 O3 2.951(8) 2_665
Na2 O3 2.951(8) .
Na2 P3 3.1676(11) 3_554
Na2 P3 3.1677(11) 3_454
Na2 P3 3.1677(11) 3_564
Na2 Ba2 3.726(4) 1_565
Na3 O2 2.387(13) 3
Na3 O2 2.387(13) 5_665
Na3 O2 2.387(13) 6_565
Na3 O6 2.581(14) .
Na3 O1 3.001(13) 3
Na3 O1 3.001(12) 6_565
Na3 O1 3.001(12) 5_665
Na3 P2 3.198(10) .
Na3 P1 3.243(2) 3
Na3 P1 3.243(2) 3_565
Na3 P1 3.243(2) 3_455
Na3 Na4 3.362(6) 3_565
Na4 O1 2.303(14) .
Na4 O1 2.303(14) 4
Na4 O1 2.303(14) 2
Na4 O2 2.337(16) 2
Na4 O2 2.337(16) 4
Na4 O2 2.337(16) .
Na4 Na1 3.261(5) 1_445
Na4 Na1 3.261(5) 1_545
Na4 Na3 3.362(6) 3_554
Na4 Na3 3.362(6) 3_444
Na4 Na3 3.362(6) 3_454
Ba1 O3 2.726(10) 6_554
Ba1 O3 2.726(10) 5_554
Ba1 O3 2.726(10) 3_554
Ba1 O1 2.870(10) 2
Ba1 O1 2.870(10) 4
Ba1 O1 2.870(10) .
Ba1 O5 3.1505(11) 3_554
Ba1 O5 3.1505(11) 3_444
Ba1 O5 3.1506(11) 3_454
Ba1 P2 3.560(4) 3_554
Ba1 P2 3.560(4) 3_444
Ba1 P2 3.560(4) 3_454
Ba2 O3 2.720(11) 2
Ba2 O3 2.720(11) 4
Ba2 O3 2.720(11) .
Ba2 O2 2.855(12) .
Ba2 O2 2.855(12) 2
Ba2 O2 2.855(12) 4
Ba2 O6 3.1487(4) 3_554
Ba2 O6 3.1487(4) 3_444
Ba2 O6 3.1487(4) 3_454
Ba2 O4 3.1534(13) 1_445
Ba2 O4 3.1534(14) .
Ba2 O4 3.1534(13) 1_545
P1 O2 1.500(14) .
P1 O2 1.500(14) 4_565
P1 O2 1.501(14) 2_665
P1 O4 1.514(19) .
P1 Na3 3.243(2) 3_554
P1 Na3 3.243(2) 3_454
P1 Na3 3.243(2) 3_564
P1 Ba2 3.581(4) 1_565
P1 Ba2 3.581(4) 1_665
P2 O5 1.52(2) .
P2 O1 1.566(11) 6_565
P2 O1 1.566(11) 3
P2 O1 1.566(11) 5_665
P2 Na12 3.170(2) 3
P2 Na12 3.170(2) 3_565
P2 Na12 3.170(2) 3_455
P2 Na1 3.355(5) 3
P2 Na1 3.355(5) 3_565
P2 Na1 3.355(5) 3_455
P2 Ba1 3.560(4) 3_565
P3 O3 1.523(6) 5_665
P3 O3 1.523(7) 3
P3 O3 1.523(6) 6_565
P3 O6 1.548(12) .
P3 Na2 3.1676(11) 3
P3 Ca2 3.1676(11) 3
P3 Na2 3.1677(11) 3_565
P3 Ca2 3.1677(11) 3_565
P3 Ca2 3.1676(11) 3_455
P3 Na2 3.1676(11) 3_455
P3 Ba2 3.548(2) 3_565
P3 Ba2 3.548(2) 3
O1 P2 1.566(11) 3_554
O1 Na12 2.333(10) 1_545
O1 Na1 2.398(10) 1_545
O1 Na3 3.001(12) 3_554
O2 Na3 2.387(13) 3_554
O3 P3 1.523(6) 3_554
O3 Ca2 2.512(7) 1_545
O3 Na2 2.512(7) 1_545
O3 Ba1 2.726(10) 3
O4 Ba2 3.1534(13) 1_565
O4 Ba2 3.1534(13) 1_665
O5 Ba1 3.1505(11) 3_565
O5 Ba1 3.1505(11) 3
O5 Ba1 3.1505(11) 3_665
O6 Ba2 3.1487(4) 3_565
O6 Ba2 3.1487(4) 3_665
O6 Ba2 3.1487(4) 3
